Europe PMC Funders Author Manuscripts

The classical and quantum dynamics of molecular spins on graphene Christian Cervetti1,*, Angelo Rettori2, Maria Gloria Pini3, Andrea Cornia4, Ana Repollés5, Fernando Luis5, Martin Dressel1, Stephan Rauschenbach6, Klaus Kern6,7, Marko Burghard6, and Lapo Bogani1,8,* 11.

Physikalisches Institut, Universität Stuttgart, Pfaffenwaldring 57, D-70550 Stuttgart (Germany) di Fisica, Università di Firenze, Via G. Sansone 1, I-50019 Sesto Fiorentino (Italy) 3Istituto dei Sistemi Complessi, CNR, Unità di Firenze, Via Madonna del Piano 10, I-50019 Sesto Fiorentino (Italy) 4Dipartimento di Scienze Chimiche e Geologiche, Università di Modena e Reggio Emilia, INSTM RU, Via G. Campi 183, I-41125 Modena (Italy) 5Instituto de Ciencia de Materiales de Aragón, CSIC-Universidad de Zaragoza, C/ Pedro Cerbuna 12, E-50009 Zaragoza (Spain) 6Max-Planck-Institut für Festkörperforschung, Heisenbergstrasse 1, D-70569 Stuttgart (Germany) 7Institut de Physique de la Matière Condensée, Ecole Polytechnique Fédérale de Lausanne (EPFL), CH-1015 Lausanne, (Switzerland) 8Department of Materials, University of Oxford, 16 Parks Road, OX1 3PH Oxford, (United Kingdom) 2Dipartimento

Abstract Europe PMC Funders Author Manuscripts

Controlling the dynamics of spins on surfaces is pivotal to the design of spintronic1 and quantum computing2 devices. Proposed schemes involve the interaction of spins with graphene to enable surface-state spintronics3,4, and electrical spin-manipulation4-11. However, the influence of the graphene environment on the spin systems has yet to be unraveled12. Here we explore the spingraphene interaction by studying the classical and quantum dynamics of molecular magnets13 on graphene. While the static spin response remains unaltered, the quantum spin dynamics and associated selection rules are profoundly modulated. The couplings to graphene phonons, to other spins, and to Dirac fermions are quantified using a newly-developed model. Coupling to Dirac electrons introduces a dominant quantum-relaxation channel that, by driving the spins over Villain’s threshold, gives rise to fully-coherent, resonant spin tunneling. Our findings provide fundamental insight into the interaction between spins and graphene, establishing the basis for electrical spin-manipulation in graphene nanodevices.

Users may view, print, copy, and download text and data-mine the content in such documents, for the purposes of academic research, subject always to the full Conditions of use:http://www.nature.com/authors/editorial_policies/license.html#terms * [email protected]. * [email protected]. Author contributions C.C. performed the functionalization and most measurements. A.C. synthetized the molecules. C.C. and S.R. acquired the MALDITOF spectra. A.R. and F.L. performed the very-low-temperature magnetic measurements. A.R., M.G.P. and L.B. performed the theoretical analysis. L.B. and M.B. conceived the experiments. L.B. wrote the draft and all authors contributed to discussions and the final manuscript. Additional information The authors declare no competing financial interests. Supplementary information (SI) accompanies this paper at www.nature.com.

Cervetti et al.

Page 2

Keywords graphene; spin dynamics; nanomaterials; quantum tunneling; molecular magnetism

Europe PMC Funders Author Manuscripts

Carbon-based spintronics offers means to manipulate localized spins in close proximity of a carbon nanotube14-16 or graphene sheet4-11. This task requires understanding and tuning the interaction between the components, in order to minimize quantum-decoherence16, and to enable spin manipulation, e.g. by controlling either the magnetic anisotropy18 or the electronic coupling5,19. Here, we exploit the exceptionally-clean magnetic features of singlemolecule-magnets (SMMs)13 to explore how spins interact with graphene substrates. The graphene-SMM hybrids are obtained by non-covalent grafting of [Fe4(L)2(dpm)6], (Hdpm=dipivaloylmethane and H3L=2-hydroxymethyl-2-(4-(pyren-1-yl)butoxy)methylpropane-1,3-diol, Fig.1a)20 via solution-based assembly onto exfoliated graphene sheets. The two pyrene groups serve as anchors20 to the graphene sheet. Functionalization of both solid-supported and bulk dispersions of graphene layers (Methods) allows determining the aggregation behaviour of the molecules on surface and performing magnetization measurements on statistically-relevant samples.

Europe PMC Funders Author Manuscripts

Atomic force microscopy (AFM) confirms successful decoration of graphene by [Fe4(L)2(dpm)6] (Fig.1b). Similar coverage was observed for single- and multi-layer graphene. Sufficiently low concentrations of [Fe4(L)2(dpm)6] (C10−5 M (SI). Multiple techniques evidence that the deposited SMMs are structurally and electronically intact. In particular, the height distribution in AFM images peaks at 1.8±0.3 nm (Fig.1c), in close agreement with the size of a single [Fe4(L)2(dpm)6] molecule.20 In addition, Raman spectra (Fig.1d) exhibit only a small up-shift of the graphene G-band by ~4 cm−1 after functionalization, indicating slight p-type doping21. This conclusion is supported by the small positive shift of the charge-neutrality-point observed in the resistance vs. gate voltage curves (Figs.1e and 1f), corresponding to a charge-transfer of only 0.08 e− per SMM. Furthermore, X-ray photoelectron spectra display the same characteristic Fe2p peak positions of thick films of [Fe4(L)2(dpm)6] (SI) and mass spectra evidence clear fingerprints of intact [Fe4(L)2(dpm)6] at 1919, 1763 and 1736 amu (Fig.1g and SI). The static magnetic properties of the hybrids are indistinguishable from those of crystalline [Fe4(L)2(dpm)6] (Fig.2). The temperature (T) dependence of the χmT curves (where χm is the static molar magnetic susceptibility, defined as the ratio between magnetization and the applied magnetic field, M/H) displays the same minimum at 100 K and a maximum around 6 K (Fig.2a, SI). The M vs H data also match within experimental error. The characteristic χmT vs T curve can be fitted20 by considering g=2.00±0.05 and two intramolecular exchange interactions between nearest-neighbour and next-nearest-neighbour Fe(III) ions (with exchange constants JNN=14.85±0.05 cm−1 and JNNN=0.09±0.05 cm−1, respectively), in excellent agreement with previous investigations, confirming a total spin ground state S=5.

Nat Mater. Author manuscript; available in PMC 2016 June 07.

Cervetti et al.

Page 3

Europe PMC Funders Author Manuscripts

The low-temperature magnetic properties of SMMs are dominated by the presence of a large magnetic anisotropy13, which partially lifts the degeneracy of the ground multiplet and creates an energy barrier ΔE separating the |ms〉 and |−ms〉 states (Fig.3a). Two spinrelaxation mechanisms are thus possible: a classical overbarrier process, where multiple phonon absorptions allow overcoming ΔE, and a quantum tunneling (QT) mechanism, which takes place between degenerate levels at opposite sides of the barrier13. QT can be suppressed by applying an external magnetic field H that lifts the degeneracy of the |±ms〉 levels. This allows examining the effect of graphene on both relaxation mechanisms separately. The magnetization dynamics is probed by measuring the real (χ′) and imaginary (χ″) response to a small magnetic field oscillating at frequency ω. In a static field H=1 kOe (Fig. 3b), where only thermally-activated behaviour is present, isolated molecules on graphene show a faster magnetization dynamics than those in crystalline [Fe4(L)2(dpm)6], for which Arrhenius analysis yields a barrier ΔE=9.7±0.7 cm−1. In H=0 (Fig.3c), all |ms〉 and |−ms〉 sublevels fall back into resonance and QT is activated, thereby magnifying enormously the differences between the hybrids and crystals response. The T-dependence of the spin relaxation time, τ, (Fig.4a) shows that for crystalline [Fe4(L)2(dpm)6] the thermallyactivated region persists down to 800 mK, below which temperature QT sets in. This contrasts strikingly with the spin relaxation in the hybrids, which is entirely dominated by QT, and the QT-rate is about one million times higher (τ−1 =105 Hz vs. 10−1 Hz). To explain these observations we subdivide the spin anisotropy into different contributions, with each term having the symmetry of a corresponding tesseral harmonic. This approach produces an intuitive but rigorous picture of the spin behaviour via the Hamiltonian:

Europe PMC Funders Author Manuscripts

(1)

where the first term describes the Zeeman interaction between the molecular spin S and H (μB is the Bohr magneton, g is the Landé factor) and the second models the spin anisotropy via the spin operators coefficient

that correspond to different harmonics, each weighted by a

. These operators, called Stevens operator-equivalents13,22 contain the jth

power of the spin ladder operators, and , and the (i-j)th power of (see SI for explicit expressions and a pictorial representation of the associated harmonics). With equation (1) we can model the effect of any external electric field, e.g. the electron density of an underlying substrate, by introducing in the sum a term of corresponding symmetry12,22 and discarding all terms not belonging to the point group of the spin environment. Stevens operatorequivalents have an effect on both classical and quantum relaxation channels:

terms with

j=0 contain powers of only, and contribute to ΔE but do not mix the |ms〉 eigenstates; terms with j≠0, on the contrary, mix states differing in ms by a multiple of j, opening the QT relaxation channel.

Nat Mater. Author manuscript; available in PMC 2016 June 07.

Cervetti et al.

Page 4

For crystalline [Fe4(L)2(dpm)6], equation (1) reads , and electron paramagnetic resonance (EPR) studies

yield20

, and g=2.000±0.005. Being

, the leading j=0 term,

Europe PMC Funders Author Manuscripts

, while multiple spectroscopic and magnetic investigations on related systems determined

to be